- Nano Express
- Open Access
Uniformly Nanopatterned Graphene Field-Effect Transistors with Enhanced Properties
© Choi et al. 2015
- Received: 26 March 2015
- Accepted: 12 June 2015
- Published: 11 July 2015
We have successfully fabricated and characterized highly uniform nanopatterned graphene (NPG). Thin anodized aluminum oxide nanomask was prepared by facile self-assembly technique without using polymer buffer layer, which was utilized as a direct-contact template for oxygen plasma etch to produce near-periodic, small-neck-width NPG. The NPG exhibits a homogeneous mesh structure with an average neck width as small as ~11 nm. The highly uniform 11-nm neck width creates a quantum confinement in NPG, which has led to a record bandgap opening of ~200 meV in graphene for the given level of neck width. Electronic characterization of single-layer NPG field-effect transistors (FETs) was performed, which demonstrated a high on-off switching ratio. We found that the NPG allows for experimental confirmation of the relationship between electrical conductance and bandgap. This work also demonstrates that our direct-contact, self-assembled mask lithography is a pathway for low-cost, high-throughput, large-scale nanomanufacturing of graphene nanodevices.
- Nanopatterned graphene
- Field-effect transistor
Graphene has recently emerged as a new and exciting 2D material due to its remarkable properties including high charge mobility, mechanical strength, and flexibility [1–3]. Potential applications of graphene as electrodes in a wide range of devices including field-effect transistors (FETs) , touch-sensitive screens , liquid-crystal displays , light-emitting diodes , dye-sensitized solar cells [8, 9], and organic solar cells  have been reported.
However, due to the semimetallic nature of graphene, it lacks a bandgap, which is necessary for technological applications such as FETs. Hence, this results in a very low on/off ratio in graphene field-effect transistor devices. For practical applications, an on/off ratio on the order of 105 is needed. One way to open a bandgap in graphene is to create geometrical constrictions of graphene material. This will lead to the confinement of electrons thus opening a bandgap. In order to increase the driving current for practical applications, such geometrical constrictions need to be maximized by fabrication of dense, ordered nanoribbon arrays, which has been achieved by electron-beam lithography [11, 12]. Although conventional lithographic methods can provide precisely located nanoarrays, the e-beam lithography is time-consuming and costly, and therefore, the size of the patterned area is often limited to the micrometer-scale regions.
To advance a facile process technique for nanopatterned graphene (NPG), we have specifically utilized an anodic aluminum oxide (AAO) lithography as it can be scaled to large-area substrates with high fidelity of patterning, which can be compatible with conventional lithographic processes [13, 14]. With an array of nanoholes introduced, the sheet resistance obviously becomes deteriorated due to a lost material pathway. Zeng et al. reported that nanometer-sized features on graphene cannot be achieved simply by directly placing the AAO membrane on reduced graphene oxide because of the rigid nature of AAO. Thus, polymethylmethacrylate (PMMA) was employed in their experiment as an adhesion layer between the AAO and graphene . In that work, graphene nanomesh (GNM) with a neck width of 14.7 nm was produced, but the low density of nanoholes and the low number of on/off ratio failed to open up the bandgap of GNM for FET operation. The use of polymer buffer/adhesion layer causes less intimate contacts of the mask with the underlying graphene surface, so the resolution of the plasma etch nanopatterning can be adversely affected. However, in the present research, we were able to overcome the issue by fabricating a less rigid and thin AAO template (~200-nm thick), and successfully demonstrated fabrication of nanohole-patterned graphene using this oxide template without polymer buffer layer thus avoiding such complicated processes. Moreover, our NPG is semiconducting in behavior with a substantially increased effective energy gap of 200 MeV at room temperature. The key to this success was the thinness and uniformity of the AAO membrane that we provided in fabrication of water-floatable AAO membranes.
Here, we report the production of a graphene nanostructure that can open up a bandgap in a large sheet of single-layer graphene (SLG). We focus on experimental investigations in SLG FETs and the implications for the device performances. The patterned graphene is prepared by self-assembled mask lithography using a floating AAO that can be placed on the device surface by lift-up of the device from underneath. Such nanostructuring process can effectively open up a conduction bandgap in a large piece of graphene, e.g., by using a several-centimeter-sized AAO membrane. We expect that the relative ease of our AAO lithography technique which can be implemented and scaled to large areas, together with the demonstrated effectiveness in controlling the electronic properties of graphene, will be useful for efforts toward practical large area, commercial applications of graphene in electronics, thin-film devices, flexible electronics, optoelectronics, and sensing.
Preparation of AAO Membrane
A 0.5-mm thick annealed Al foil purchased from Alfar Aesar (99.99 %) was used as the starting material. The Al foil was successively degreased by acetone and isopropyl alcohol with ultrasonication, followed by deionized (DI) water rinse and nitrogen gas blow. The Al foil was slightly etched in a 1 M NaOH aqueous solution to remove any possible surface contaminations prior to surface-smoothing electropolishing process conducted at 20 V in a solution of perchloric acid (70 %) and ethanol (99.9 %) (1:4 volume ratio) at 5 °C for 15 min, using a Pt counter electrode. Then, a two-step anodization process of the Al foil was carried out by incorporating the Al foil as the working electrode and Pt as the counter electrode, immersed in 0.3-m oxalic acid. The electrolyte temperature was maintained at 1 °C during the anodization process using a powerful refrigeration bath (RTE7, Thermo Scientific) in which the coolant circulates a double-wall glass chamber. After the first anodizing process, which took about 3 h at an operating voltage of 40 V, the anodized Al foil was immersed for 1 h in a mixed solution of phosphoric acid (6 wt%) and chromic acid (1.8 wt%) kept at 75 °C to remove the alumina layer formed in the first anodizing step. The second anodizing step was implemented for 10 min while other experimental conditions were unchanged compared with the first anodizing step, in order to form an ordered porous alumina membrane on the Al foil. Then, the Al metallic substrate underneath the AAO layer was selectively removed with a mixed HCl and CuCl2 solution for 10 min. Any residual Cu debris adhered to the bottom of the AAO barrier layer was removed by placing the sample in nitric acid for a few seconds and washed in DI water immediately after. The barrier layer in the bottom of the AAO holes was then removed by a 5 wt% phosphoric acid etching for 10 min to 2 h.
Fabrication of NPG
A single-layer graphene was purchased from ACS material (MA, USA). Before graphene on Cu backing layer was separated and transferred to other substrates, the back side of graphene was first removed by oxygen plasma. The top side of graphene was protected by a PMMA layer coating during the O2 plasma etching. The graphene film was then transferred onto a 300-nm SiO2-coated Si substrate (Si/SiO2) using chemical processing steps. The chemical process for graphene transfer consists of the etching of Cu foil, transferring the floating graphene onto a Si/SiO2 substrate by lift-up in an aqueous solution bath, followed by washing with water, acetone, and isopropyl alcohol as described elsewhere . After that, the PMMA layer was removed by dissolving it in acetone. Furthermore, the rapid thermal annealing was carried out for graphene placed on the Si/SiO2 substrate by heating to 400 °C under a N2 atmosphere to remove the residual PMMA and promote the adhesion between graphene and the oxide layer.
The prepared AAO template floating in water was placed on the graphene as an etch mask by lifting up the Si/SiO2 substrate from underneath. After that, the sample was annealed in a vacuum at 180 °C for 2 h, in order to allow the AAO membrane to stick tightly on the graphene surface. Then, oxygen plasma (30 W, 150 mTorr) was applied through the AAO template holes to etch and create pores on the graphene. The details of recipes and procedures for the formation of NPG were explained in previous study .
The sample microstructure was characterized by ultra-high resolution scanning electron microscopy (UHR SEM; FEI XL30). Raman spectroscopy was used as a nondestructive tool for probing the edges and the crystalline sp2-bonded structure of the graphene . Raman spectra were collected using a Renishaw Raman spectrometer inbuilt with an Ar+ laser of a wavelength of 514 nm for quantifying the degree of structural order and charge transfer characteristics. To measure the sheet resistance of graphene nanomesh (GNM), Jandel Four-Point Probe was employed for the four-point measurement. The optical property of the graphene samples was characterized by UV/Vis spectrophotometer (UNICO SQ-4802).
We have achieved the current on/off ratio values significantly higher than those in the previously reported FET devices of graphene nanoribbon (GNR) and graphene nanomesh (GNM) [21–25]. The expected bandgap from the relation of E g ~ α/w by an average neck width of ~10 nm was 95 MeV. In Fig. 5d, however, the actual bandgap in our FET device with an 11-nm neck-width NPG is estimated to be ~200 MeV from Eq. (2) with our measured I on/I off value of 50. By contrast, the FET device with a larger 25-nm neck-width NPG exhibits an order of magnitude smaller I on/I off ratio of ~5.3 with much less bandgap opening as shown in Fig. 5. There is a difference between the calculated bandgap values from the relations with the neck width of our FET having an average neck width of ~11 nm and the on/off current ratio experimentally measured, with the actual measured ratio being higher. Further detailed study is in progress to understand the mechanism behind this observation of surprisingly highly effective bandgap in our NPG samples. We assume that the unusually high on/off ratio in our more extensively patterned graphene affected the bandgap opening, possibly due to the highly dense and uniform NPG nanostructure throughout the large-area samples. Such results point to a possibility of utilizing the properly and highly uniformly nanopatterned large-area graphene as promising electronic devices [26, 27].
Electrical characterization of NPG confirmed that the current on-off ratio is inversely proportional with the neck width, indicating the formation of an effective gap due to the confinement effect. We have shown that both electronic transport and Raman characteristics change in a concerted manner on graphene patterning. The availability of such well-controlled NPG structure will provide an interesting possibility for a more in-depth fundamental investigation of transport behavior in the highly interconnected graphene network, and will enable exciting opportunities in sensitive electronics and sensor devices.
We demonstrate a successful fabrication of very fine dimension NPG using a thin-floating anodic aluminum oxide (AAO) membrane etching mask. The membrane was directly transferred onto a hydrophobic graphene surface for well-adhered and stacked manner on the graphene due to the van der Waals force, thus allowing a high-density, small-neck-width NPG structure fabrication, without using any intermediate buffer/adhesion polymer which could adversely affect the resolution of plasma etching patterning of graphene. The NPG so produced exhibits homogeneous mesh structures with an average neck width as small as ~11 nm. Electronic characterization of a single-layer NPG FET structure with an 11-nm neck width creates a quantum confinement in NPG, which has led to an impressive bandgap opening of ~200 MeV. The NPG structures with different neck widths allowed experimental confirmation of the relationship between electrical conductance and bandgap. Electrical characterization of the NPG-based FET device confirmed that the current on/off ratio is inversely proportional with the neck width, indicating the formation of an effective gap due to a confinement effect. The availability of such NPG will provide an interesting system for a more in-depth fundamental investigation of transport behavior in the highly interconnected, small-width graphene network and will enable exciting opportunities in sensitive electronic or sensor devices. This work also demonstrates that self-assembled mask lithography is a pathway for low-cost, high-throughput, large-scale nanomanufacturing of NPG with critical dimensions down to nanometer regime.
The authors wish to acknowledge the financial support from Iwama endowed fund at UC San Diego.
- Park CH, Yang L, Son YW, Cohen ML, Louie SG. Anisotropic behaviors of massless Dirac fermions in graphene under periodic potentials. Nat Phys. 2008;4:213–7.View ArticleGoogle Scholar
- Bolotin KI, Sikes KJ, Jiang Z, Klima M, Fudenberg G, Hone J, et al. Ultrahigh electron mobility in suspended graphene. Solid State Commun. 2008;146:351–5.View ArticleGoogle Scholar
- Choi W, Lahiri I, Seelaboyna R, Kang Y. Synthesis of graphene and its applications: a review. Crit Rev Solid State Mater Sci. 2010;35:52–71.View ArticleGoogle Scholar
- Castro NAH, Guinea F, Peres NMR, Novoselov KS, Geim AK. The electronic properties of graphene. Rev Mod Phys. 2009;81:109–62.View ArticleGoogle Scholar
- Kim M, Safron NS, Han E, Arnold MS, Gopalan P. Fabrication and characterization of large-area, semiconducting nanoperforated graphene materials. Nano Let. 2010;10:1125–31.View ArticleGoogle Scholar
- Son YW, Cohen ML, Louie SG. Half-metallic graphene nanoribbons. Nature. 2006;444:347–9.View ArticleGoogle Scholar
- Ferrari AC. Raman spectroscopy of graphene and graphite: disorder, electron-phonon coupling, doping and nonadiabatic effects. Solid State Commun. 2007;143:47–57.View ArticleGoogle Scholar
- Das S, Sudhagar P, Ito E, Lee DY, Nagarajan S, Lee SY, et al. Effect of HNO3 functionalization on large scale graphene for enhanced tri-iodide reduction in dye-sensitized solar cells. J of Mater Chem. 2012;22:20490–7.View ArticleGoogle Scholar
- Das S, Sudhagar P, Verma V, Song D, Ito E, Lee SY, et al. Amplifying charge-transfer characteristics of graphene for triiodide reduction in dye-sensitized solar cells. Adv Funct Mater. 2011;21:3729–36.View ArticleGoogle Scholar
- Berger C, Song ZM, Li XB, Wu XS, Brown N, Naud C, et al. Electronic confinement and coherence in patterned epitaxial graphene. Science. 2006;312:1191–6.View ArticleGoogle Scholar
- Lu W, Lieber CM. Nanoelectronics from the bottom up. Nature Mater. 2007;6:841–50.View ArticleGoogle Scholar
- Wang X, Dai H. Etching and narrowing of graphene from the edges. Nature Chem. 2010;2:661–5.View ArticleGoogle Scholar
- Choi D, Kuru C, Choi C, Noh K, Hong SK, Das S, et al. Nanopatterned graphene field effect transistor fabricated using block co-polymer lithography. Mater Research Lett. 2014;2:131–9.View ArticleGoogle Scholar
- Zeng Z, Huang X, Yin Y, Li H, Chen Y, Li H, et al. Fabrication of graphene nanomesh by using an anodic aluminum oxide membrane as a template. Adv Mater. 2012;24:4138–42.View ArticleGoogle Scholar
- Zhang YB, Tang TT, Girit C, Hao Z, Martin MC, Zettl A, et al. Direct observation of a widely tunable bandgap in bilayer graphene. Nature. 2009;459:820–3.View ArticleGoogle Scholar
- Gupta A, Chen G, Joshi P, Tadigadapa S, Eklund PC. Raman scattering from high-frequency phonons in supported n-graphene layer films. Nano Lett. 2006;6:2667–73.View ArticleGoogle Scholar
- Malard LM, Pimenta MA, Dresselhaus G, Dresselhaus MS. Raman spectroscopy in graphene. Phys Rep. 2009;473:51–87.View ArticleGoogle Scholar
- Cancado LG, Jorio A, Ferreira EHM, Stavale F, Achete CA, Capaz RB, et al. Quantifying defects in graphene via Raman spectroscopy at different excitation energies. Nano Lett. 2011;11:3190–6.View ArticleGoogle Scholar
- Ryu S, Maultzsch J, Han MY, Kim P, Brus LE. Raman spectroscopy of lithographically patterned graphene nanoribbons. Acs Nano. 2011;5:4123–30.View ArticleGoogle Scholar
- Ozyilmaz B, Jarillo-Herrero P, Efetov D, Kim P. Electronic transport in locally gated graphene nanoconstrictions. Appl Phys Lett. 2007;91:192107.View ArticleGoogle Scholar
- Kosynkin DV, Higginbotham AL, Sinitskii A, Lomeda JR, Dimiev A, Price BK, et al. Longitudinal unzipping of carbon nanotubes to form graphene nanoribbons. Nature. 2009;458:872–6.View ArticleGoogle Scholar
- Bai JW, Zhong X, Jiang S, Huang Y, Duan XF. Graphene nanomesh. Nat Nanotechnol. 2010;5:190–4.View ArticleGoogle Scholar
- Li XL, Wang XR, Zhang L, Lee SW, Dai HJ. Chemically derived, ultrasmooth graphene nanoribbon semiconductors. Science. 2008;319:1229–332.View ArticleGoogle Scholar
- Wang XR, Ouyang YJ, Li XL, Wang HL, Guo J, Dai HJ. Room-temperature all-semiconducting sub-10-nm graphene nanoribbon field-effect transistors. Phys Rev Lett. 2008;100:206803.View ArticleGoogle Scholar
- Bai JW, Duan XF, Huang Y. Rational fabrication of graphene nanoribbons using a nanowire etch mask. Nano Lett. 2009;9:2083–7.View ArticleGoogle Scholar
- Choi D, Kuru C, Choi C, Noh K, Hwang S, Choi W. Unusually High Optical Transparency in Hexagonal Nanopatterned Graphene with Enhanced Conductivity by Chemical Doping. Small. doi:10.1002/smll.201402784
- Chen TL, Ghosh DS, Marchena M, Osmond J, Pruneri V. Nanopatterned graphene on a polymer substrate by a direct peel-off technique. ACS Appl Mater Interfaces. 2015;7:5938–43.View ArticleGoogle Scholar
This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/4.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly credited.